Transparent polycrystalline cubic spinels protect and .Transparent polycrystalline cubic spinels
Embed Size (px)
Transcript of Transparent polycrystalline cubic spinels protect and .Transparent polycrystalline cubic spinels
By Mohan Ramisetty, Suri Sastri, Uday Kashalikar, Lee M. Goldman, and Nagrendra Nag
Left: Spinel crystal structure. Right: Transparent aluminum oxynitride window manufactured by Surmet Corp. (Burlington, Mass.).
T he first reported work on trans-parent polycrystalline ceramics goes back to the 1950s. For example, some of the literature on materials discussed in this article, magnesium aluminate spinel and aluminum oxynitride spinels, traces back to late 1950s and early 1960s.13 The advantages of these materials over current state-of-the-art materials include
Ease of manufacturing; Superior mechanical properties, such as modulus, hard-
ness, and strength; Performance at high-temperature environments; and Chemical durability.Candidate polycrystalline transparent ceramic composi-
tions include yttrium aluminum garnet and yttria, but alumi-num oxynitride (-AlON )and magnesium aluminate spinels seem to have established themselves as leading candidates in multiple market segments, such as the military, aerospace, and lasers, mainly because of their durability, availability in large sizes, and cost.
Today, -AlON and magnesium-spinel are manufactured in large sizes and in large volumes. However, high cost remains a barrier to their deployment as replacements for glasses and some opaque ceramics. Growing demand in cur-rent and emerging markets position these materials at the
cusp of new commercialization opportunities in terms of vol-umes and costs. This article reviews the unique properties of these materials that make solving the production challenges a worthwhile endeavor.
Optical properties Properties drive applications, and, obviously, optical prop-
erties are among the most important for transparent polycrys-talline ceramics. However, the combination of mechanical properties (and, for some applications,4 other properties, too) makes these spinel materials uniquely suitable for a range of applications in defense and aerospace systems.
Many defense and aerospace applications require materials that are transparent in the ultraviolet, visible, and through the mid-infrared wavelength ranges. High transparency means low scattering losses, low reflectance, and low absorp-tion. For cubic spinel polycrystalline materials, several factors determine optical quality. Cubic materials are isotropic, so they have no inherent birefringence. However, secondary phases, such as pores, impurities, and inclusions, typically lead to low transmittance. Controlling material purity and processing conditions minimizes defects, and increases trans-parency up to theoretical limits. In the absence of absorption and scatter, reflection losses from the material's inherent refractive index determine transmittance.Consequently, transmittance can be increased significantly via antireflec-tion coatings.
Figure 1 shows transmittance of -AlON and magnesium-spinel optical ceramics. Even though it is polycrystalline, -AlON is one of the best currently available materials in terms of optical quality. The transmittance of -AlON approaches its theoretical values in the near-UV, visible through mid-IR wavelengths, but starts dropping around 4.5 micrometers and cuts off at mid-IR range wavelengths of about 6 micrometers because of intrinsic (phonon) absorp-tion. Additionally, it drops to zero at about 0.22 micrometers in the short wavelength range. In comparison, magnesium-spinel transmits further in the mid-IR rangetransmit-tance starts dropping around 5 micrometers and stops at 6.5 micrometers wavelength. The transmittance of magnesium-spinel also drops to zero at about 0.2 micrometers. This is an
With their manufacturing problems solved, the many desirable
properties of the polycrystalline transparent ceramics -AlON and
magnesium-spinel have led to many military and commercial
Transparent polycrystalline cubic spinels protect and defend
www.ceramics.org | American Ceramic Society Bulletin, Vol. 92, No. 220
21American Ceramic Society Bulletin, Vol. 92, No. 2 | www.ceramics.org
advantage for spinel applications that require high transmission in the 4.55 micrometer range.
In addition to excellent transmit-tance, commercial -AlON products have exceptional optical clarity (exceeding 98 percent) and very low haze (less than 2 percent) in the visible wavelengths. (Optical clarity relates to the amount of light scattered at small angles. In contrast, haze relates to the amount of light scattered at large angles.)
Pores, secondary phases, inclusions, defects, and inhomogeneous grain boundaries greatly affect the clar-ity and haze properties of transparent polycrystalline ceramic materials. High clarity and low haze requires nearly 100 percent density and no secondary phases, which are very challenging from a processing perspective. In addition, impurities can impart a tint to the final component, whereas less than full den-sity causes haze. Thus, the production of high-quality transparent ceramics demands both careful powder synthesis and close control during densification.
Another important optical property is the refractive index. In -AlON, it varies between 1.81 and 1.67 over the 0.45.0 micrometer wavelength range, with normal dispersion as shown in Figure 2. (Dispersion is the change in refractive index with wavelength for a material and is denoted by the dimen-sionless "Abbe number.") A typical Abbe value for -AlON and magne-sium-spinel is about 60, which means that the dispersion is much lower than some of the glasses with similar refrac-tive indices, making the spinels strong candidate materials for lenses with low chromatic aberration.
Also, the cubic spinel phase of alu-minum oxynitride exists across a wide composition range. Therefore, proper-ties, such as refractive index, can be tailored without losing transparency. Components like graded refractive index lenses (GRIN) are fabricated, for example, by controlling composition or by adding dopants. Unlike many glass-es, which are transparent only in visible wavelengths, -AlON GRIN lenses are transparent in the visible through mid-
IR range. Certain GRIN lenses can have flat surfaces, because the lens curve is built into the material via the refractive index gra-dient. Also, grading the composition can eliminate the aberra-tion associated with spherical lenses. Additionally, GRIN lenses can reduce significantly the size, weight, and com-plexity of the optical train for defense applications, such as image systems for laser range finders, night vision goggles, and unmanned aerial vehicles.
Night vision technologies improve visibility (transmission) in low light conditions. Most night vision devices (NVD) are for military applications, but some are used in the civilian arena. NVDs require transmission in the 0.40.92 micrometer range. In this range, -AlON and magnesium-spinel transmit better than glasses. As Figure 3 shows, -AlON-based armor offers significantly more night vision capability (about 4050 percent more transmission) over glass laminates in low-light conditions. More transmission means a higher signal-to-noise ratio and higher-resolution imaging, which improve awareness for the warfighter in low-light situations.
alone is not enough for warfare situations. These materials must endure stresses encountered in manufacturing, transport to the-ater, deployment in service, or ulti-mately, under bal-listic conditions. Ballistic properties and environmental
durability are critically important prop-erties in the military context.
Although -AlON and magnesium-spinel are cubic spinel lattices, their bonding and bond strength differences make -AlON mechanically superior to magnesium-spinel, giving it a higher hardness and elastic modulus than magnesium-spinel. In fact, the hardness of -AlON approaches that of single-crystal sapphire, making it the hardest polycrystalline transparent material currently available commercially. The combination of high hardness and elastic modulus makes -AlON a lead-ing candidate material for transpar-ent armor applications, followed by magnesium-spinel and single-crystal sapphire. Table 2 compares the impor-tant mechanical properties of the two transparent polycrystalline materials as well as some of their thermal properties.
Although lower elastic modulus and
Figure 1. Calculated transmittance of -AlON and magnesium-spinel (at 2 millimeter thickness). The calculation includes Fresnel reflective losses that can be eliminated through use of an antireflection coating.
Table 1. Important optical properties of transparent polycrystalline spinels
Property -AlON Mg-spinel Unit
Refractive index (at wavelength 0.5 m)6 1.80 1.723 dn/dT (in 35 m wavelength range)6 3 3 106 K1
Absorption coefficient (at 3.39 m wavelength)6 0.1 0.018 cm1
Total integrated optical scatter (at 0.64 m; ~5 mm thick 2.1 7.2 % sample)6
Transmission wavelength range* 0.226 0.256.5 m Optical homogeneity achieved in 15 in. 3 25 in. part with ~5 N/A ppm 3.4 in. aperture Typical transmittance without AR coatings (in the visible >84 7580 % range)* Typical haze (in the visible range)* 95 %
*Varies depending on thickness and processing conditions.
www.ceramics.org | American Ceramic Society Bulletin, Vol. 92, No. 222
Transparent polycrystalline cubic spinels protect and defend
hardness values of magnesium-spinel compared with those of -AlON are related to structure and bonding, the lower flexure strength is also strongly affected by processing influences. Lithium f